Received: 6 April 2017 Accepted: 6 July 2017 Published: xx xx xxxx
Observation of the unexpected morphology of graphene wrinkle on copper substrate Wen Wang1, Shudu Yang2 & Ashu Wang3 Graphene, a two-dimensional material, has a wide range of unique properties and could be used in the development of varieties of mechanic, electronic and photonic devices, therefore methods to synthesis large-area high-quality graphene films are urgently required. Chemical vapor deposition (CVD) has been of particular interest recently due to its simplicity and low cost. However, because of the mismatch of thermal expansion coefficients, high densities of wrinkles are commonly observed. Despite their prevalence and potential impact on large-scale graphene properties, relatively little is known about their structural morphology and formation mechanism. In this article, morphologies of graphene obtained by CVD are experimentally investigated by an atomic force microscope (AFM) and results show that the profiles of wrinkles are much larger than they should be. By using theoretical methods and molecular dynamics simulations (MD), we find internal molecules created during CVD process which supply additional pressure is the main mechanism. Graphene as a two-dimensional (2D) material has many unique physical and mechanical properties, including highest strength, elastic stiffness, in-plane electrical conductivity and thermal conductivity1–5. Graphene is widely supposed to be a material to enable new development of many modern technologies4, 6 which involves the potential applications in mechanic, electronic and photonic devices7–10. However, wrinkling is a ubiquitous phenomenon in 2D membranes that severely weaken the performance of graphene. In spite of very fast improving methods on manufacturing graphene, a large-area high-quality wrinkle-free graphene has yet to emerge. The practical difficulty to use graphene in devices is that the available methods for growing graphene contain high density of wrinkles11. Systematically understand the mechanism of wrinkle formation can help controlling its morphology and further eliminating wrinkles. Due to its low cost and efficiency, CVD has been widely adopted to manufacture graphene. A particular issue for graphene obtained by CVD is the presence of high density of wrinkles. These are formed by differential thermal expansions, as the metal contracts more than the graphene during cooling process, leaving an excess area of graphene12–15. Despite their prevalence and potential impact on large-scale graphene properties, relatively little is known about their structural morphology and formation mechanism16, 17. In this letter, we use AFM to characterize surface morphology of graphene wrinkles and find morphology of graphene wrinkles measured by AFM is not real. The widths of wrinkle are much wider than theory and simulation results that cannot be understood. By using MD simulations and theoretical methods, we quantitatively studied the unexpected mechanism of wrinkles.
Experiment details. Single layer graphene samples were obtained by CVD methods18 which were grew on
copper foil substrate at temperatures up to 1000 °C. Generally copper foil has a positive thermal expansion coefficient of 16.5 × 10−6/K, however, graphene has an negative in-plane thermal expansion coefficient of −8 × 10−6/K19. This contrast leads to a compression strain about 2.45% between graphene films and copper substrate after reduced to room temperature. The binding between graphene and copper is weak and graphene can slip on copper surface20, 21, as a consequence the strain distribution is no longer uniform, typically, wrinkles can be easily found in large strain areas. In order to obtain more quantitative morphological information about wrinkles, AFM in tapping mode was adopted to investigate profiles of wrinkles. We first used conventional AFM tips with the typical diameter of ~10 nm in tapping mode to measure heights and widths of graphene wrinkle. We measured 10 1
School of Mechanical Engineering, Southwest Jiaotong University, Chengdu, 610031, China. 2Sichuan Branch of Meteorological Training Institute CMA, Chengdu, 610072, China. 3School of Information Science and Engineering, Chengdu University, Chengdu, 610106, China. Correspondence and requests for materials should be addressed to W.W. (email: [email protected]
) or A.W. (email: [email protected]
) ScIEntIfIc REPOrtS | 7: 8244 | DOI:10.1038/s41598-017-08159-8
Figure 1. Experimental AFM morphology image of graphene wrinkles on copper sustrate by using super-sharp and high resolution tips. (a,c) AFM morphology image of graphene wrinkles obtained by CVD methods. (b,d) The AFM heights of the cross-sectionl trace of the line marked in Fig. 1a and c respectively.
graphene wrinkles, the typical measured profiles can be found in Fig. S1. Experimental measurement results show that widths of graphene wrinkles are in the range of tens of nanometers and with heights in the range of a few nanometers. Considering the fact that the width of wrinkles and the radius of tips are in the same order, shapes of AFM tips may have effect on the accuracy of wrinkle’s morphologies22. To avoid the effect and obtain more accurate profiles of graphene wrinkles, high resolution super sharp tips (Hi’Res-C14/Cr-AU from Micromasch) with tip spike radius of ~1 nm and spike height 100–200 nm are used in the paper. Figure 1a and c show the AFM morphological images of typical graphene wrinkles scanned in tapping mode. Total 8 graphene wrinkle were measured. The AFM heights of the the cross-sectionl trace of the line marked in Fig. 1a and c are shown in Fig. 1b and d respectively. Experimental measurements clearly show that widths of graphene wrinkles are 30 nm ≤ 2 W ≤ 40 nm, heights of graphene wrinkles are 3.4 nm ≤ h ≤ 11 nm. The profiles of wrinkles in the article are consistent with the previous results16 but the unexpected morphologies and mechanisms are not clear.
Theory analysis without interlayer molecules. The binding energy (Γ)23 between graphene foil and
copper substrate can be used to verify the accuracy of the measured morphology. We do this in the framework of the elastic theory, generalized to account for bending energy (Eb) and adhesion energy (Ea). In this model, the total energy consists of two parts: the bending energy stored in the graphene and the adhesion energy that represents the atomic interactions (binding) between graphene and copper substrate. The only unknown inputs to the model are the height and width of wrinkles. According to the measured results, profiles of wrinkles can be reasonably assumed to satisfy ys = 1 h(1 + cos( πx )) 2 W W /2 Dbh 2π4 and Eb can be simply written as Eb = Db ∫ , where D = 1.2 eV = 0.192 nN·nm24 is the bending (y ′ )2 dx = 2 −W /2 s 16W 3 stiffness graphene, b represents length of wrinkle along its axis, h is height of wrinkles and W is half width of wrinkles. The adhesion energy (Ea) between graphene and copper can be calculated as Ea = bΓW, where Γ represents the binding energy between graphene and copper per unit area. In the equilibrium state Eb−Ea = 0. By using the experimental measurements of h and W, the obtained adhesion energy Γ ≤ 0.0034 J/m2. Recently, Γ has been determined by experiments and first principle calculations. The reported value 0.397 J/m2 ≤Γ ≤ 0.72 J/m2 20, 21, which is at least 2 orders of magnitude large than the results we estimated. These observations, taken together, clearly demonstrate that the profiles of graphene wrinkles measured by AFM are not real, however, little is known about the factors determining the profiles of wrinkles so far. Morphologies may depend on the process of CVD growth and environment; however, previous studies haven’t already yielded insight into the mechanism. To better understand the unexpected morphology of graphene wrinkles, we performed several MD simulations to help understanding the machanism. The model itself is a stack of a rectangular copper substrate (red
ScIEntIfIc REPOrtS | 7: 8244 | DOI:10.1038/s41598-017-08159-8
Figure 2. MD simulation models and calculated results, T = 300 K. (a) The MD simulation model is a stack of two rectangular materials, upper cyan graphene and lower red copper. (b) After the pre-compression being released, a typical graphene wrinkle is clearly formed on copper substrate. (c) Simulation results of graphene wrinkles vesus strain, for small strain, both h and W increase with strain; for large strain, h still increases with strain, however, W surprisingly decreses with strain. The error bars represent the standard deviation of five independent calculations.
Figure 3. Typical cross-sectional shape of graphene wrinkles under different strain obtained by MD simulation (T = 300 K) and the comparison between theory and simulation results. (a) Typical cross-sectional shape of graphene wrinkles under strain form 12% to 65%. (b) Comparison to the simulation results, the theory fit and predict the results well. The error bars represent the standard deviation of five independent calculations for the same model.
part in Fig. 2a) and a single layer graphene (cyan part in Fig. 2a), with the basal planes of both parallel. In order to obtain wrinkles, a pre-compressive strain was applied to graphene layer. Then a horizontal spring with stiffnes k = 100 eV/Å2 was applied to each end of graphene in order to fix the both ends. Finally the whole model were relaxed under a constant tempereture T = 300 K, as a result, many wrinkles with variety of profiles were formed on copper substrate. Wrinkles are formed by differential thermal expansions, as the metal substrate contracts more than the graphene during cooling process. So it should form uniform random distribution wrinkles, however, the binding between graphene and copper is weak and graphene can slip on copper surface, as a consequence the strain distribution is no longer uniform which leads to non-uniform distribution of wrinkles. This phenomenon was confirmed by scanning electron microscopy images in supplementary Fig. S2(a). We observed that neighbored wrinkles can merge to form larger wrinkles in the MD simulation, see supplementary Fig. S2(b)–(d). There is a large strain of graphene in the area containing wrinkles and small strain in the area without wrinkles. What’s more, the copper substrates used in CVD growth are polycrystalline with various thickness, defects and crystal orientations which leads to very large local strain. Base on the upper phenomenon, we can conclude that wrinkles are formed by two processes. At first, high density of small wrinkles with ripple structure are formed due to thermal compression strain. Second, if there are no pining between graphene and copper substrate, neighbored wrinkles merged to form wrinkles with large strain mushroom structure and thus decrease density of wrinkles. In the MD calculations, strain is defined as ε = ΔW/W (see insert of Fig. 3b), where W is the flat graphene length without forming wrinkle and ΔW represents the difference of wrinkle’s width and length of flat graphene. Because of the merge of wrinkles and Fig. 2b shows a typical obtained graphene wrinkle on copper with strain ɛ = 17.7%. Here we systematicaly invetigated morphology of graphene wrinkles under different strains
ScIEntIfIc REPOrtS | 7: 8244 | DOI:10.1038/s41598-017-08159-8
www.nature.com/scientificreports/ (T = 300 K, 12.4%